Download presentation

Presentation is loading. Please wait.

Published byEmerald Brown Modified about 1 year ago

1
Bulk Topological Superconductor

2
Z Possible Topological Superconductors Time-Reversal Invariant (TRI) Time-Reversal Broken (TRB) 1D 2D 3D Z2Z2 Z2Z2 Z2Z2 Z - Schnyder-Ryu-Furusaki-Ludwig (2008) Kitaev (2009) “Periodic Table” of topological invariant Chiral p-wave SC in TI surface Surface State of TIs Bogoliubov qp EFEF TI SC = 0 = 0 = = Fu & Kane (2008) EFEF 22 Majorana Edge State Sr 2 RuO 4 (D) (DIII)

3
Z Possible Topological Superconductors Time-Reversal Invariant (TRI) Time-Reversal Broken (TRB) 1D 2D 3D Z2Z2 Z2Z2 Z2Z2 Z - Schnyder-Ryu-Furusaki-Ludwig (2008) Kitaev (2009) “Periodic Table” of topological invariant Kitaev model 1D Nanowire of InSb or InAs Majorana End-State Alicea, RPP (2012) Oreg et al., PRL (2010) Lutchyn et al., PRL (2010) Chiral p-wave SC in TI surface Mourik et al., Science (2012) Das et al., Nature Phys. (2012) InSb/ NbTiN InAs/Al (D) (DIII)

4
Z Possible Topological Superconductors Time-Reversal Invariant (TRI) Time-Reversal Broken (TRB) 1D 2D 3D Z2Z2 Z2Z2 Z2Z2 Z - Schnyder-Ryu-Furusaki-Ludwig (2008) Kitaev (2009) “Periodic Table” of topological invariant Kitaev model Superfluid 3 He-B phase The surface state may host Helical Majorana Fermions that are itinerant and massless E kyky EFEF New 3D topological state of matter Chiral p-wave SC in TI surface (D) (DIII)

5
SC in Cu x Bi 2 Se 3 Hor et al., PRL (2010) Conventional SC State in the bulk Proximity SC E k EFEF Topological SC State in the bulk Fu & Berg, PRL (2010) E k EFEF Helical Majorana fermions Four-component Hamiltonian of Bi 2 Se 3 with the basis ( P1 z + , P1 z + , P2 z - , P2 z - ) Majorana zero mode in vortices Hosur et al., PRL (2011)

6
SC in Cu x Bi 2 Se 3 Hor et al., PRL (2010) Conventional SC State in the bulk Proximity SC E k EFEF Topological SC State in the bulk Fu & Berg, PRL (2010) E k EFEF Helical Majorana fermions Zero Resistivity Specific Heat Jump SC V.F. 70% Problem: Sample is difficult to prepare, shielding fraction is low. Majorana zero mode in vortices Hosur et al., PRL (2011)

7
SEM image of an actual sample (Ag particle size ~50 nm) Sasaki, Ando et al., PRL (2011) Ag particles on the surface “Soft” Point Contact Sn Cu x Bi 2 Se 3 T-dep. B-dep.

8
Effects of Heating and/or Critical Currents? Example of a spurious ZBCP G(V)/G n V (mV) 0 0 T 0.5 T 0.75 T 1 T Sheet et al., PRB (2004) Dip position moves with H Peak height is insensitive to H T = 0.35 K H dependence is completely different! H-dep. Reflectionless tunneling would be governed by L ~ 1 m and suppressed with ~1 mT. Andreev bound state due to an unconventional SC state

9
Possible SC States in Cu x Bi 2 Se 3 Four-component Hamiltonian of Bi 2 Se 3 ( P1 z + , P1 z + , P2 z - , P2 z - ) Sasaki, Ando et al., PRL (2011) All odd-parity states are topologically non-trivial and host helical Majorana fermions on the surface Fu & Berg, PRL (2010)

10
Unconventional SC States in Cu x Bi 2 Se 3 2 : Odd parity, full gap 4 ( 3 ) : Odd parity, point node Helical Majorana A Hsieh & Fu, PRL(2012) Helical Majorana B Helical Majorana C Yamakage et al., PRB (2012) dI/dV for A dI/dV for B dI/dV Sasaki, Ando et al., PRL (2011) ZBCP due to helical Majorana fermions?

11
Conventional s-wave ? Controversy in Cu x Bi 2 Se 3 STM Levy et al., PRL (2013) If the bulk is BCS s-wave Parity mixing of pair potential is anomalously enhanced by surface Dirac fermions EFEF Mizushima, Yamakage, Sato & Tanaka, PRB (2014) Opening of an additional surface gap which is larger than the bulk gap ?

12
Controversy in Cu x Bi 2 Se 3 n cm cm cm -3 Lahoud et al., PRB (2013) n = 2 cm -3 n = 4 cm -3 Levy et al., PRL (2013) Quasi-2D TSC? Mizushima et al., arXiv:

13
Superconducting Doped TCI

14
Topological Crystalline Insulator SnTe SnTe Hsieh et al., Nature Commun. (2012) PbTe SnTe : contribution from Te p-orbital SnTe PbTe Band inversion + Mirror symmetry Nontrivial Mirror Chern number kyky 0 kxkx Z 2 invariant = 0 Tanaka, Sato, Ando et al., Nature Physics (2012)

15
In-doped SnTe Superconductor n = 2 – 8 cm -3 Sn 1-x In x Te Erickson et al., PRB (2009) Ferro- electric NaCl Structure Te 2- Sn 2+ /In 3+ Sato, Ando et al., PRL (2013) Topological SS is present in Sn 1-x In x Te. RhombohedralCubic Novak, Ando et al., PRB (2013)

16
In-doped SnTe Sn 1-x In x Te (x = 0.045) B- dep. T c = 1.2 K Faceted (001) surface T- dep meV 2 Peak suppression corresponds to H c2 Normalized ZBCP height is > 2 !! Surface Andreev Bound State due to Unconventional SC Point-Contact Spectroscopy Sasaki, Fu, Ando et al., PRL (2012)

17
SnTe vs. PbTe SnTe PbTe Tanaka, Ando et al., Nature Phys. (2012) T- dep. Sn 1-x In x Te Pb 1-x Tl x Te Conventional Similar FS structures, but the band parities are different. Unconventional

18
Possible SC States in Sn 1-x In x Te k p Hamiltonian of SnTe around each L point z = 1 p orbitals of Sn and Te with opposite parity ( k 3 : along L, k 1 : along LK ) Possible Pairing Symmetry (representations of D 3d group) Parity A 1g A 1u A 2u EuEu even odd Topologically non-trivial Topological SC? k p Hamiltonian of Bi 2 Se 3 around point z = 1 Se p z orbitals on the top and bottom layer Sasaki, Fu, Ando et al., PRL (2012)

19
Possible SC States in Sn 1-x In x Te Possible Pairing Symmetry (representations of D 3d group) Parity A 1g A 1u A 2u EuEu even odd Topologically non-trivial RhombohedralCubic Novak, Ando et al., PRB (2013) Topological SC? Sasaki, Fu, Ando et al., PRL (2012)

20
Majorana Zero Mode in Vortices? Cu x Bi 2 Se 3 Majorana zero mode in vortices Hosur et al., PRL (2011) Sn 1-x In x Te Multiple Majorana zero modes can coexist due to additional symmetry to protect them from hybridization If the bulk SC is conventional:

21
Natural Heterostructure

22
Natural Heterostructure PSBS [(PbSe) 5 ] n [(Bi 2 Se 3 ) 3 ] m n = 1 m = 1 m = 2 m = (Bi 2 Se 3 ) “Quintuple Layer” Nakayama, Sato, Ando et al., PRL (2012)

23
Natural Heterostructure PSBS Y. Zhang, Q.K. Xue et al., Nat. Phys. (2010) m = 1 m = 2 m = Surface states are encapsulated by the insulating PbSe layer Quasi-2D system with topological “bulk” state !! “Surface states” in every (Bi 2 Se 3 ) m units? Ultra-thin Bi 2 Se 3 Films Nakayama, Sato, Ando et al., PRL (2012)

24
Cu-intercalation to PSBS m = 2 Sasaki, Segawa, Ando, PRB (2014)

25
Nearly 100% Volume Fraction Specific-heat behavior is very different from BCS, suggesting a gap with line nodes Sasaki, Segawa, Ando PRB (2014)

26
Reproducibility C el (T) is reproducible in two high-volume-fraction samples. Sasaki, Segawa, Ando PRB (2014)

27
Magnetic-Field Dependence of C el Sasaki, Segawa, Ando PRB (2014)

28
Implications of Cu-PSBS Nodal Gap Unconventional SC None of the previously known superconducting TI presented clear bulk signature of unconventional SC Sign Changing Gap + Strong Spin-Orbit Coupling Spin-split surface Andreev bound state (i.e. Helical Majorana fermions) Quasi 2D-Fermi surface Majoranas are on the side surface or terrace edge d-wave gap

29
SrPtAs

30

31
Stronger relaxation in the SC state Appearance of spontaneous magnetic field TRS breaking T-dependence of penetration depth Full gap d+id (chiral d-wave) pairing ?

32
Thank you!

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google